Principles of Cathodic Protection
Comprehensive information on CP system...
4.18 Principles of Cathodic Protection V. Ashworth This article is a revision of the Third Edition article 10.1 by V. Ashworth, volume 2, pp 10:3–10:28, ß 2010 Elsevier B.V.
4.18.1 4.18.2 188.8.131.52 184.108.40.206 220.127.116.11 18.104.22.168 4.18.3 22.214.171.124 126.96.36.199 4.18.4 188.8.131.52 184.108.40.206 220.127.116.11 18.104.22.168 4.18.5 4.18.6 4.18.7 4.18.8 4.18.9 References
Historical Background Electrochemical Principles Aqueous Corrosion Cathodic Protection Oxygen Reduction Hydrogen Evolution Methods of Applying Cathodic Protection Impressed Current Method Sacrificial Anodes Proof of Protection Steel Other Metals Steel in Concrete Potential Measurements Current Requirements Coatings and Cathodic Protection Calcareous Deposit Potential Attenuation in Impressed-Current Systems Summary
Abbreviations AC Alternating current BS British Standard DC Direct current emf Electromotive force EN European Norm NACE National Association of Corrosion Engineers SRB Sulfate-reducing bacteria
Symbols E Potential E Equilibrium potential Ea Anodic potential Ec Cathodic potential Ecorr Corrosion potential I Current Ia Anodic current Ic Cathodic current Icorr Corrosion current Ilim Limiting current
2747 2748 2748 2748 2749 2750 2751 2751 2752 2753 2753 2755 2755 2756 2757 2758 2759 2759 2761 2762
IR Ohmic drop (equivalent to a voltage) R Resistance h Overpotential
4.18.1 Historical Background In recent years, it has been regarded as somewhat passe´ to refer to Sir Humphry Davy in a text on cathodic protection. However, his role in the application of cathodic protection should not be ignored. In 1824, Davy presented a series of papers to the Royal Society in London,1 in which he described how zinc and iron anodes could be used to prevent the corrosion of copper sheathing on the wooden hulls of British naval vessels. His paper shows a considerable intuitive awareness of what are now accepted as the principles of cathodic protection. Several practical tests were made on vessels in harbor and on seagoing ships, including the effect of various current densities on the level of protection of the copper. Davy also considered the use of an impressed current
device based on a battery, but did not consider the method to be practicable. The first ‘full-hull’ installation on a vessel in service was applied to the frigate HMS Samarang in 1824. Four groups of cast iron anodes were fitted, and virtually perfect protection of the copper was achieved. So effective was the system that the prevention of corrosion of the copper resulted in the loss of the copper ions required to act as a toxicide for marine growth, leading to increased marine fouling of the hull. Since this led to some loss of performance from the vessel, interest in cathodic protection waned. The beneficial action of the copper ions in preventing fouling was judged to be more important than preventing deterioration of the sheathing. Cathodic protection was therefore neglected for 100 years, after which it began to be used successfully by oil companies in the United States to protect underground pipelines.2 It is interesting that the first large-scale application of cathodic protection by Davy was directed at protecting copper rather than steel. It is also a measure of Davy’s grasp of the topic that he was able to consider the use of two techniques of cathodic protection, namely sacrificial anodes and impressed current, and two types of sacrificial anode, namely zinc and cast iron.
4.18.2 Electrochemical Principles 22.214.171.124
The aqueous corrosion of iron under conditions of air access can be written as 2Fe þ O2 þ 2H2 O ! 2FeðOHÞ2
The product, ferrous hydroxide, is commonly further oxidized to magnetite (Fe3O4) or a hydrated ferric oxide (FeOOH), that is, rust. It is convenient to consider separately the metallic and nonmetallic reactions in eqn : 2Fe ! 2Fe
O2 þ 2H2 O þ 4e ! 4OH
schematic representation of aqueous corrosion occurring at a metal surface. Equation , which involves consumption of the metal and release of electrons, is termed an anodic reaction. Equation , which represents consumption of electrons and dissolved species in the environment, is termed a cathodic reaction. Whenever spontaneous corrosion reactions occur, all the electrons released in the anodic reaction are consumed in the cathodic reaction; no excess or deficiency is found. Moreover, the metal normally takes up a more or less uniform electrode potential, often called the corrosion or mixed potential (Ecorr). 126.96.36.199
It is possible to envisage what might happen if an electrical intervention was made in the corrosion reaction by considering the impact on the anodic and cathodic reactions. For example, if electrons were withdrawn from the metal surface, it might be anticipated that reaction  would speed up (to replace the lost electrons) and reaction  would slow down, because of the existing shortfall of electrons. It follows that the rate of metal consumption would increase. By contrast, if additional electrons were introduced at the metal surface, the cathodic reaction would speed up (to consume the electrons) and the anodic reaction would be inhibited; metal dissolution would be slowed down. This is the basis of cathodic protection. Figure 2 shows the effect on the corrosion reaction shown in Figure 1 of providing a limited supply of electrons to the surface. The rate of dissolution O2 + 2H2O
To balance eqns  and  in terms of electrical charge, it has been necessary to add four electrons to the right-hand side of eqn  and to the left-hand side of eqn . However, simple addition and rationalization of eqns  and  yield eqn . We conclude that corrosion is a chemical reaction  occurring by an electrochemical mechanism (eqns  and ), that is, by a process involving electrical and chemical species. Figure 1 is a
Fe Metal (iron or steel)
Figure 1 Schematic illustration of the corrosion of steel in an aerated environment. Note that the electrons released in the anodic reaction are consumed quantitatively in the cathodic reaction, and that the anodic and cathodic products may react to produce Fe(OH)2.
Principles of Cathodic Protection
slows down because the external source rather than an iron atom provides two of the electrons. Figure 3 shows the effect of a greater electron supply; corrosion ceases since the external source provides all the requisite electrons. It should be apparent that there is no reason why further electrons could not be supplied, when even more hydroxyl (OH) ion would be produced, but without the possibility of a concomitant reduction in the rate of iron dissolution. Clearly, this would be a wasteful exercise. The corrosion reaction may also be represented on a polarization diagram (Figure 4). The diagram O2 + 2H2O
Metal From external source
Figure 2 Schematic illustration of partial cathodic protection of steel in an aerated environment. Note that one of the anodic reactions shown in Figure 1 has been annihilated by providing two electrons from an external source; an excess of OH ions over Fe2þ now exists at the surface.
O2 + 2H2O
Environment 4OH– Fe
Fe 4e From external source
Figure 3 Schematic illustration of full cathodic protection of steel in an aerated environment. Note that both anodic reactions shown in Figure 1 have now been annihilated, and there is an accumulation of OH at the surface.
shows how the rates of the anodic and cathodic reactions (both expressed in terms of current flow I) vary with electrode potential E. Thus, at Ea, the net rate of the anodic reaction is zero and it increases as the potential becomes more positive. At Ec, the net rate of the cathodic reaction is zero and it increases as the potential becomes more negative. (To be able to represent the anodic and cathodic reaction rates on the same axis, the modulus of the current has been drawn.) The two reaction rates are electrically equivalent at Ecorr, the corrosion potential, and the corresponding current Icorr is an electrical representation of the rate of the anodic and cathodic reactions at that potential, that is, the spontaneous corrosion rate of the metal. That is, at Ecorr the polarization diagram represents the situation referred to above; namely, that when spontaneous corrosion occurs, the rate of electron release equals the rate of electron consumption, and there is no net current flow although metal is consumed, and meanwhile the metal exerts a single electrode potential. To hold the metal at any potential other than Ecorr requires that electrons be supplied to, or be withdrawn from, the metal surface. For example, at E 0 , the cathodic reaction rate I 0 c, exceeds the anodic reaction rate I 0 a, and the latter does not provide sufficient electrons to satisfy the former. If the metal is to be maintained at E 0 , the shortfall of electrons given by (|I 0 c| – I 0 a) must be supplied from an external source. This externally supplied current serves to reduce the metal dissolution rate from Icorr to I 0 a. At Ea, the net anodic reaction rate is zero (there is no metal dissolution) and a cathodic current equal to I 00 c must be available from the external source to maintain the metal at this potential. It may also be apparent from Figure 4 that, if the potential is maintained below Ea, the metal dissolution rate remains zero (Ia ¼ 0), but a cathodic current greater than I 00 c must be supplied; more current is supplied without achieving a benefit in terms of metal loss. There will, however, be a higher interfacial hydroxyl ion concentration. 188.8.131.52
In illustrating the corrosion reaction in eqn , the oxygen reduction reaction  has been taken as the cathodic process. Moreover, in Figures 1–4, oxygen reduction has been assumed. While there is a range of cathodic reactions that can provoke the corrosion of a metal (since to be a cathodic reactant, any particular species must simply act as an oxidizing
Ec Fe2+ + 2e
O2 + 2H2O + 4e
|I⬘⬘c | log [ I ] Figure 4 Polarization diagram representing corrosion and cathodic protection. A corroding metal takes up the potential Ecorr spontaneously and corrodes at a rate given by Icorr. If the potential is to be lowered to E0 , a current equal to (|I 0 c| – I 0 a) must be supplied from an external source; the metal will then dissolve at a rate equal to I 0 a.
agent to the metal), the most common cathodic reactant present in natural environments is oxygen. It is for this reason that the oxygen reduction reaction has been emphasized here. When corrosion occurs, if the cathodic reactant is in plentiful supply, it can be shown both theoretically and practically that the cathodic kinetics are semilogarithmic, as shown in Figure 4. The rate of the cathodic reaction is governed by the rate at which electrical charge can be transferred at the metal surface. Such a process responds to changes in electrode potential, giving rise to the semilogarithmic behavior. Because oxygen is not very soluble in aqueous solutions (10 ppm in cool seawater, for example), it is not freely available at the metal surface. As a result, it is often easier to transfer electrical charge at the surface than for oxygen to reach the surface to take part in the charge transfer reaction. The cathodic reaction rate is then controlled by the rate of arrival of oxygen at the surface. This is often referred to as mass transfer control. Since oxygen is an uncharged species, its rate of arrival is unaffected by the prevailing electrical field and responds only to the local oxygen concentration gradient. If the cathodic reaction is driven so fast that the interfacial oxygen concentration is reduced to zero (i.e., the oxygen is consumed as soon as it reaches the surface), the oxygen concentration gradient to the surface reaches a maximum and the reaction rate attains a limiting value. Only an increase in oxygen concentration or an increase in flow velocity will permit an increase in the limiting value. The cathodic kinetics under mass transfer control will be as shown in Figure 5.
Fe2+ + 2e
E Ecorr E⬘ Ea
|I⬘c | |Ic⬘⬘| = Ilim = Icorr O2 + 2H2O + 4e
log [ i ] Figure 5 Polarization diagram representing corrosion and cathodic protection when the cathodic process is under mass transfer control. The values of Ecorr and Icorr are lower than when there is no mass transfer restriction, that is, when the cathodic kinetics follows the dotted line.
Figure 5 demonstrates that, even when semilogarithmic cathodic kinetics is not observed, partial or total cathodic protection is possible. Indeed, Figure 5 shows that the corrosion rate approximates to the limiting current for oxygen reduction (Ilim), and the current required for protection is substantially lower than when semilogarithmic cathodic behavior prevails. 184.108.40.206
In principle, it is possible for water to act as a cathodic reactant with the formation of molecular hydrogen: 2H2 O þ 2e ! H2 þ 2OH
Principles of Cathodic Protection
Indeed, in neutral solutions, the corrosion of iron with concomitant hydrogen evolution deriving from the reduction of water is thermodynamically feasible. In practice, this cathodic reaction is barely significant because the reduction of any oxygen present is both thermodynamically favored and kinetically easier. In the absence of oxygen, the hydrogen evolution reaction at the corrosion potential of iron is so sluggish that the corrosion rate of the iron is vanishingly small. Nevertheless, hydrogen evolution is important in considering the cathodic protection of steel. Although hydrogen evolution takes little part in the corrosion of steel in aerated neutral solutions (see Figure 6), as the potential is lowered to achieve cathodic protection, it plays a larger, and eventually dominant, role in determining the total current demand. This too is demonstrated in Figure 6 where, it must be remembered, the current supplied from the external source at any potential must be sufficient to sustain the total cathodic reaction, that is, both oxygen reduction and hydrogen evolution reactions at that potential. It will be seen that to lower the potential much below Ea entails a substantial increase in current and significantly more hydrogen evolution.
4.18.3 Methods of Applying Cathodic Protection There are two principal methods of applying cathodic protection, namely the impressed current technique and the use of sacrificial anodes. EC
O2 + 2H2O + 4e
The former includes the structure as part of a driven electrochemical cell, and the latter includes the structure as part of a spontaneous galvanic cell. 220.127.116.11
Impressed Current Method
Figure 7 illustrates the use of an external power supply to provide the cathodic polarization of the structure. The circuit comprises the power source, an auxiliary or impressed current electrode, the corrosive solution, and the structure to be protected. The power source drives a positive current from the impressed current electrode through the corrosive solution and onto the structure. The structure is thereby cathodically polarized (its potential is lowered), and the positive current returns through the circuit to the power supply. Thus, to achieve cathodic protection, the impressed current electrode and the structure must be in both electrolytic and electronic contact. The power supply is usually a transformer/rectifier that converts AC power to DC. Typically, the DC output will be in the range 15–100 V and 5–100 A, although 200 V/200 A units are not unknown. Thus, fairly substantial driving voltages and currents are available. Where mains power is not available, diesel or gas engines, solar panels, or thermoelectric generators have all been used to provide suitable DC. It will be seen that the impressed current electrode discharges positive current, that is, it acts as an anode in the cell. There are three generic types of anode used in cathodic protection, namely consumable, nonconsumable, and semiconsumable. The consumable electrodes undergo an anodic reaction that involves their consumption. Thus, an anode made of scrap iron produces positive current by the reaction
Fe ! Fe2þ þ 2e
2+ + 2e
+ DC power – Electron flow source
Ecorr |I⬘C |
2H2O + 2e
2OH– + H2
Figure 6 Polarization diagram showing the limited role hydrogen evolution plays at the corrosion potential of steel in aerated neutral solution, the larger role in determining cathodic protection currents, and the dominant role in contributing to current requirements at very negative potentials. The dotted line shows the total cathodic current due to oxygen reduction and hydrogen evolution.
Impressedcurrent anode in ground bed
Positive current flow (ionic)
Figure 7 Schematic diagram of cathodic protection using the impressed-current technique.
The ferrous ions then enter the environment as a positive current carrier (although in practice the current will be carried in the environment by aqueous ions such as Naþ and Cl. Since the dissolving anode must obey Faraday’s law, it follows that the wasting of the anode will be proportional to the total current delivered. In practice, the loss for an iron anode is approximately 9 kg A1 year1. Thus, consumable anodes must be replaced at intervals, or be of sufficient size to remain as a current source for the design life of the protected structure. This poses some problems in design because, as the anode dissolves, the resistance it presents to the circuit increases. More important, it is difficult to ensure continuous electrical connection to the dissolving anode. Nonconsumable anodes sustain an anodic reaction that decomposes the aqueous environment rather than dissolves the anode metal. In aqueous solutions the reaction may be 2H2 O ! O2 þ 4Hþ þ e or in the presence of chloride ions 2Cl ! Cl2 þ 2e Anodes made from platinized titanium or niobium belong to this category. Because these anodes are not consumed faradaically, they should not, in principle, require replacement during the life of the structure. However, to remain intact, they must be chemically resistant to their anodic products (acid and chlorine) and, where the products are gaseous, conditions must be produced that allow the gas to escape and not interfere with anode operation. This is particularly true of the platinized electrodes because they can operate at high current density (>100 A m2) without detriment, but will then produce high levels of acidity (pH < 2) and large volumes of gas. Ground-bed design (the way in which the anode is installed) is therefore crucial. Although the anodes are described as nonconsumable, they do suffer some loss of the thin (2.5–10 mg m3) platinized coating. This loss, which unfortunately has become known as the wear rate although there is no question of the loss being due to mechanical wear, is usually small, related to the total current passed, and increased if the applied current has an AC component. Typically, values for the loss rate are 8 mg A1 year1 for platinized titanium, which may be increased 10-fold if an AC component of